Forensic Glass Analysis. Characteristics of Glass. Hard, amorphous solid Usually transparent Primarily composed of silica, with various amounts of elemental oxides Brittle Exhibits conchoidal fracture. Common Types.
Hard, amorphous solid
Primarily composed of silica, with various amounts of elemental oxides
Exhibits conchoidal fracture
Soda-lime—used in plate and window glass, glass containers, and electric lightbulbs
Soda-lead—fine tableware and art objects
Borosilicate—heat-resistant, like Pyrex
Silica—used in chemical ware
Tempered—used in side windows of cars
Laminated—used in the windshield of most cars
Density—mass divided by volume
Refractive index (RI)—the measure of light bending due to a change in velocity when traveling from one medium to another
Markings—striations, dimples, etc.
Immersion method—lower fragments into liquids whose refractive index is different
Match point—when the refractive index of the glass is equal to that of the liquid
Becke line—a halo-like glow that appears around an object immersed in a liquid. It disappears when the refractive index of the liquid matches the refractive index of the object (the match point).
Determination of Refractive Index, continued
The refractive index of a high-boiling liquid, usually a silicone oil, changes with temperature.
This occurs in an apparatus called a hot stage which is attached to a microscope. Increasing the temperature allows the disappearance of the Becke line to be observed.
At match point, temperature is noted and refractive index of the liquid is read from a calibration chart.
The Becke line is a “halo” that can be seen on the inside of the glass on the left, indicating that the glass has a higher refractive index than the liquid medium. The Becke line as seen on the right is on the outside of the glass, indicating just the opposite.
Radial fracture lines radiate out from the origin of the impact; they begin on the opposite side of the force.
Concentric fracture lines are circular lines around the point of impact; they begin on the same side as the force.
3R rule—Radial cracks form a right angle on the reverse side of the force.
A high-velocity projectile always leaves a wider hole at the exit side of the glass.
Cracks terminate at intersections with others. This can be used to determine the order in which the fractures occurred.
Class characteristics: physical and chemical properties such as refractive index, density, color, chemical composition
Individual characteristics: if the fragments can fit together like pieces of a puzzle, the source can be considered unique
The collector must consider that fragments within a questioned sample may have multiple origins. If possible, the collector should attempt an initial separation based on physical properties.
The collector must consider the possibility that there may be a physical match to a known sample (e.g., a piece of glass to a fractured vehicle headlamp). When an attempt to make a physical match is made at the site of collection, the collector should take precautions to avoid mixing of the known and questioned samples.
Any glass samples collected should be documented, marked (if necessary), packaged, and labeled.
—Forensic Science Communications
The glass sample should consist of the largest amount that can be practically collected from each broken object and packaged separately. The sample should be removed from the structure (e.g., window frame, light assembly). The inside and outside surfaces of the known sample should be labeled if a determination of direction of breakage or reconstruction of the pane is desired.
When multiple broken glass sources are identified, it is necessary to sample all sources.
A sample should be collected from various locations throughout the broken portion of the object in order to be as representative as possible.
The sample should be collected with consideration being given to the presence of other types of evidence on that sample (e.g., fibers, blood).
—Forensic Science Communications